A novel method to correct for wood MOE ultrasonics and NIRS measurements on increment cores in Liquidambar styraciflua L
Ultrasounds overestimate the MOE value. This paper analyses the causes of this difference and opens the perspective for a novel method allowing the calculation of the correct MOE from ultrasounds or NIRS measurements on cores.
Standardized methods for determining wood modulus of elasticity (MOE) are destructive and require many replicates. Other methods such as NIRS and ultrasound have been developed to characterize wood properties and overcome these constraints.
The aim of this study was to compare the two MOE measurement methods (NIRS and ultrasound) applied to cores of wood taken from standing trees (Liquidambar styraciflua).
MOE, measured by an acoustic method in standard samples (360 × 20 × 20 mm), was used as a reference. Then MOE was predicted by an NIRS model and determined using ultrasound in standard samples (360 × 20 × 20 mm), small samples (10 × 20 × 20 mm), and cores (15 mm in diameter).
MOE values determined by acoustic method on standard samples and by ultrasonic method on small samples were correlated (R2 = 0.72) and were not statistically different. The NIRS PLS regression yielded a model with R2cv = 0.80. The link between NIRS and ultrasound on cores was statistically significant (R2 = 0.68).
The ultrasonic technique determines an apparent modulus enables comparative data analysis. This apparent modulus can be used for quantitative analysis if a corrective model is used. A correction formula to ultrasonic MOE was proposed in the case of a prismatic geometry.
KeywordsLiquidambar styraciflua Near infrared spectrometry Ultrasonic measurement Modulus of elasticity Cores of wood
The determination of modulus of elasticity (MOE) by standardized methods is time-consuming and requires large quantities of plant material. These methods are generally destructive for the test sample or the tree given that sample extraction requires its felling. Standardized methods therefore cannot be used to monitor changes in MOE during a tree’s growth even though such information is important for the future use of its wood. An alternative technique is to use small samples such as cores. Previous studies (Perrin and Ferrand 1984; Bucur 1981, 1986; Nepveu 1988; Pelletier et al. 2008) have shown that it is possible to determine shrinkage, growth stress, and MOE using cores taken from standing trees. MOE can be determined in cores by ultrasonic or near infrared spectrometry (NIRS) assessment. The studies conducted by Schimleck et al (2003), Baillères et al (2002); Schimleck and Evans (2004), Hein et al (2010), Chaix et al (2010), Leblon et al (2013), and Tsuchikawa and Schwanninger (2013) showed that NIRS is useful for predicting certain physico-mechanical properties of wood. Bucur (1981) conducted ultrasonic measurements on 5-mm-diameter cores. More recent wood science studies (Brancheriau 2013; Ozyhar et al. 2013; Xu and Wang 2014) have improved ultrasonic measurement of MOE but the results obtained were not compared with those of standardized tests or other non-destructive methods. In order to measure MOE on increment cores, the study described herein aimed to (i) compare MOE values determined by the ultrasonic method with values obtained by modal analysis of flexural vibrations, (ii) identify the optimal model for determining MOE by near infrared spectrometry, and (iii) compare MOE values obtained using the ultrasonic method with those determined by NIRS.
2 Materials and methods
2.1 Study materials
This study is focused on Liquidambar styraciflua, a hardwood species of American origin. This species may be of interest for local wood markets in Madagascar because of its technological characteristics and color (American Hardwood Export Council 2008). L. styraciflua accounts for 30 % of hardwood stocks in southern USA (Carter and Hughes 1984). The wood of this species is highly popular on American and European wood markets, especially for the production of pallets, paneling, or furniture, because of its suitability for staining and finishing (American Hardwood Export Council 2008 and 2009). The success of this species is attributed not only to its wood, but also to its great plasticity. L. styraciflua has a high potential to adapt to different environmental conditions and can be managed by coppicing from the stump (Colonado 1992). In addition, this species is fast growing and has great ability to colonize wasteland (Sabistina 2010). Finally, its abundant seeds multiply easily in the nursery and can be stored in cool dry environments without any decrease in germination potential for about 3 years (Bonner 1970). Based on this potential, L. styraciflua is of great interest for Madagascar because it fulfills the requirements of the Malagasy wood market (fast-growing species, multi-purpose wood, high plasticity, and relatively resistant to the passage of fire) (Chaix and Ramamonjisoa 2001).
As part of an international provenance trial on L. styraciflua, the Oxford Commonwealth Forestry Institute shipped Liquidambar seeds to Madagascar from 13 provenances mainly within the natural area of the species distribution, i.e., southeastern USA, Mexico, and Central America. These 13 Liquidambar provenances of were introduced at Mandraka (Madagascar) in 1986. Fifty-four 23- to 24 year-old trees were subsequently felled for thinning purposes. They were derived from the nine best provenances in terms of height and diameter. Two sampling areas were selected (foot of slope and ridge) to maximize the variability of the characters under study. Prismatic bars (N = 201, 360 × 20 × 20 mm in L, R, T planes) were then cut from quartersawn boards. In addition, 99 radial cores (15 mm diameter and 378 mm mean length) were taken from the dominant trees (25 years old). All samples were stabilized at 20 °C, 65 % RH.
2.2 Experimental procedure
2.3 Free flexural vibration tests
The sample was placed on two elastic mountings (vibration deflection on the L-T plane). A steel ball (diameter 13 mm; weight 9 g) was used to create an impact on one end of the bar and a laser vibrometer was placed at the other end. The sound generated was filtered (analogic filtering with frequency cut-off at 10 kHz) and then digitalized with 12-bit resolution. The acquisition parameters were set to ensure a frequency resolution of ±1.35 Hz (first resonance frequency close to 790 Hz). The first three frequencies were used to determine the MOE A based on Bordonné’s solution to Timoshenko’s theory (Brancheriau 2002).
2.4 Ultrasound measurements
Emission and acquisition settings were specific to the length of the tested sample: square signal for five periods and time resolution of ±0.2 μs (0.3 % error for the propagation time determined in a 360 mm sample); ± 0.05 μs pulse signal and time resolution (2.5 % error for the propagation time determined in a 10 mm sample). As the MOE US error was greater for small samples, the mean of triplicate measurements/results was used. Theoretically, 70 repetitions would be required to reduce the error to 0.3 %, but only three repetitions were performed given the high number of measurements.
2.5 Near infrared spectrometry measurements
Near infrared spectra were taken on the radial tangential plane of the prismatic bars. Chaix et al (2010) showed that regression models yield accurate predictions when measurements are made on this plane. A Bruker Vector 22/N spectrophotometer combined with OPUS version 5.0 software was used in diffuse reflectance mode with a sintered gold standard as reference. This Fourier transform spectrophotometer is designed for reflectance analysis of solids and contains an integrating sphere. The same instrument with the same control software was then used with the same settings to measure absorption spectra of the cores, again in the radial tangential plane. Spectra were acquired over a 12,500 to 3500 cm−1 (800 to 2850 nm) range at 8 cm−1 resolution. Each spectrum was made up of 2335 absorption values, and 16 scans were averaged for each spectrum to improve the signal-to-noise ratio.
2.6 Calibration of the near infrared spectrometry regression model
2.7 Data processing
3.1 Comparison of acoustic and ultrasonic methods used on prismatic bars
Comparison of mean MOE values determined by acoustic and ultrasonic methods (N = 21)
3.2 Comparison of the NIRS model and ultrasonic method used on cores
Descriptive statistics for MOE values determined by ultrasonic (US) and NIRS methods on cores (N = 1801)
4.1 Acoustic and ultrasonic methods
Numerical error values were as follows: Δm = ±0.1 g (m = 95 g for L = 360 mm and m = 2.6 g for L = 10 mm); Δh = Δw = ±0.1 mm (h = w = 20 mm); ΔL = ±1 mm (L = 360 mm) and ΔL = ±0.1 mm (L = 10 mm); Δτ = ±0.2 μs (τ = 74.6 μs for L = 360 mm); and Δτ = ±0.05 μs (τ = 2.07 μs for L = 10 mm). Theoretical uncertainty in this case was 1.9 % for a 360 mm sample and 10.6 % for a 10 mm sample. The measurement errors were acceptable and within the same order of magnitude as those associated with normalized 3- or 4-point static bending tests. Brancheriau et al (2002) reported a measurement error of 9 % for the 3-point bending test and 6 % for the 4-point bend test on 360 × 20 × 20 mm samples.
Effect of sample length on MOE values determined by the ultrasonic method
Relative difference (%)
Beech (Bucur 1981)
MOE (360 × 20 × 20 mm) > MOE core (5 mm)
MOE (360 × 20 × 20 mm) > MOE (10 × 20 × 20 mm)
MOE (360 × 20 × 20 mm) > MOE (20 × 20 × 20 mm)
In the present case, the directions (X, Y, and Z) in Eq. (8) are collinear to the wood axes (L, T, and R). This equation was used to study the effect of the (L/h) ratio on the determined MOE values (Table 3). Values attributed to the Poisson coefficients were drawn from Guitard (1987) for so-called “standard” hardwood. The true MOE value is assumed to be that obtained by the acoustic method. In the simulation, the MOE of a 360 mm prismatic bar was compared with that of a 20 mm prismatic bar (not a 10 mm bar as in our study) as the model was used within its valid range. The theoretical difference in this case is 23 %, which is consistent with the experimental values. Note that for a (L/h) ratio above 7, the apparent MOE calculated from the conventional Eq. (1) no longer varies and converges toward the true MOE value.
4.2 NIRS model
The NIRS model developed is comparable to models described in the literature for Eucalyptus species (which have technological properties similar to those of Liquidambar) and other species. Schimleck et al (2001) calibrated a model for Eucalyptus delegatensis and obtained an R2cv of 0.90 (in cross-validation). Kothiyal and Raturi (2011) obtained an R2 of 0.82 for Eucalyptus tereticornis (independent validation method with a performance to deviation ratio of 2.3). Most woods of the Eucalyptus genus have higher quantities of extractives than Liquidambar (Chein et al 2013; Rakotovololonalimanana 2013). Extractives have a major impact on the quality of NIRS models as the absorption spectra obtained are dependent upon the chemical composition of the wood and the covalent bonds therein (Schwanninger et al 2011). The fact that the quality of the model developed here was deemed to be only “fairly good” may be explained by the low levels of extractives in the test wood. Moreover, Narayanamurti et al (1962) reported that extractives have effects on the physico-mechanical properties of wood. The linear relation in Fig. 4 shows bias between the ultrasonic method and the NIRS predictive model. The NIRS model was calibrated with moduli determined by flexural vibration tests (MOE A). The ultrasonic test determined apparent moduli (Eq. 1) using the density and a propagation speed which depended on the frequency of the travelling wave (dispersion phenomenon, Brancheriau 2011). The apparent modulus was thus a function of the MOE, Poisson coefficients, and sample geometry (Eq. 8) but also of the material viscosity (the dispersion was due to the antagonist effects of viscosity and Poisson effect). The difference between moduli determined from vibration frequencies in bending and moduli determined from temporal vibrations in compression could explain the bias observed in Fig. 4. This bias could also be due to the age and quality of the trees from which the samples were taken since the samples intended for the acoustic measurements (reference measurements for the NIRS model) were taken from 23- to 24-year-old thinning trees whereas the cores were taken from dominant or co-dominant 25-year-old trees. Several previous studies (Maeglin 1987; Zobel and Buijtenen 1989; Jeffries 2008) confirmed that the tree age has an impact on the physico-mechanical properties of the wood.
The MOE values were determined by flexural vibrations (acoustic technique) and ultrasound on bars (360 × 20 × 20 mm) and small samples (10 × 20 × 20 mm). When these values were compared, a significant difference was noted between the acoustic and ultrasound findings on bars but there was no difference between acoustic values on bars and ultrasound values on small samples. The near infrared spectrometry model was obtained on bars based on the acoustic technique. This regression model was characterized by a prediction error of 1234 MPa. The associated performance to deviation ratio of 2.6 allowed us to use the model to predict MOE on cores. The ultrasound and NIRS techniques were compared on cores (linear regression on 1801 measurements). The standard error of the linear regression was in agreement with the determination error of the two techniques. A bias was however revealed by the regression, which highlighted a difference between ultrasound and NIRS (acoustic technique). The acoustic technique determined a MOE theoretically equivalent to that of a 4-point bending test (local modulus). The ultrasonic technique determined an apparent MOE mainly function of the MOE value, geometry, and Poisson coefficients for small samples. The use of ultrasound on cores is, however, possible because this leads to direct determination of the apparent MOE. Another advantage is that ultrasound could be used on small-diameter cores (3 mm). The present analysis proposed a correction formula to MOE obtained by ultrasounds in the case of a prismatic geometry. For complex geometries such as cores, the validity of the ultrasonic MOE correction should be verified using finite element analysis in order to allow for comparison with results from other studies that report on true static MOE.
We thank S Lotte (CIRAD Ur BioWooEB) and instrument makers for machining wood samples, P Gallet and S Paradis (CIRAD Ur BioWooEB) for improving Us-Scan software, Honoré Randrianjafy and Hery Rakotondraoelina (DRFP/FOFIFA Madagascar) for providing material, LMGC (Laboratoire de Mécanique et Genie Civil) team, P Langbour, and D Guibal (CIRAD Ur BioWooEB) for providing technical support.
Sample collection was funded by Centre de Coopération Internationale en Recherche Agronomique pour le Développement (CIRAD) in Montpellier, France and Département de Recherche Forestière et Piscicole (DRFP/FOFIFA) in Antananarivo, Madagascar. Laboratory work was funded by CIRAD. The main author received a grant from Agence Universitaire de la Francophonie during the 3 years of his PhD from 2011 to 2013. His PhD work was thereafter cofunded by CIRAD.
- American Hardwood Export Council (2008) Sustainable American hardwood, a guide to species, p. 40Google Scholar
- American Hardwood Export Council (2009) The illustrated guide to American hardwood lumber grades. National Hardwood Lumber Association, p. 24Google Scholar
- Bertrand D (2005) Etalonnage multidimensionnel : application aux données spectrales. Techniques de l’IngénieurGoogle Scholar
- Bonner FT (1970) Artificial ripening of sweetgum seeds. Tree Planters Notes 21:23–25Google Scholar
- Brancheriau L (2002) Expertise mécanique des sciages par analyses des vibrations dans le domaine acoustique. Thèse de l’Université de la méditerranée – Aix Marseille II, Ecole Supérieure de Mécanique de Marseille. p. 267Google Scholar
- Brancheriau L (2011) Corrections for poisson effect in longitudinal vibrations and shearing deformations in transverse vibrations applied to a prismatic orthotropic body in mechanical vibrations: types, testing and analysis, Amy L. Galloway (Ed.) Nova Science Publishers, ISBN-13: 978-1616682170, 205-223Google Scholar
- Brancheriau L (2013) Caractérisation acoustique et ultrasonore des produits bois et composites. Habilitation à diriger des recherches, dossier de synthèse. Académie de Montpellier, Université de Montpellier 2, Information Structures et Systèmes, p.122Google Scholar
- Burns DA, Ciurczak EW (2008) Handbook of near infrared analysis, (3rd edition). CRC PressGoogle Scholar
- Carter PM, Hughes CE (1984) Liquidambar styraciflua L.—a species of potential for the tropics. Commonw For Rev 63:207–216Google Scholar
- Chaix G, Ramamonjisoa L (2001) Production de semences pour les reboisements malgaches. Bois et Forêts des Tropiques 268:49–64Google Scholar
- Chaix G, Kokutse AD, Ratovomboahangy B, Guibal D, Randrianjafy H, Rakotondraoelina H, Brancheriau L, Rakotovololonalimanana H, Hein PRG, Ramananantoandro T (2010) Prediction of radial and tangential shrinkages by near infrared spectroscopy: an example for Tectona grandis from Togo and for Liquidambar styraciflua from Madagascar. Cerne 16:66–73Google Scholar
- Chein S-C, Xiao J-h, Tseng Y-H, Kuo Y-H, Wang S-Y (2013) Composition and fungial activity of balsam from Liquidambar farmosana Hance. Holzforschung 67:645–351Google Scholar
- Colonado M (1992) Liquidambar styraciflua, Fire Effects Information System. U S Department of Agriculture, Forest Service, p. 9Google Scholar
- R Development Core Team 2012 R: A language and environment for statistical computing. R Foundation for Statistical Computing, Vienna, Austria. http://www.R-project.org/
- Giordanengo T, Charpentier J-P, Boizot N, Roussel S, Roger J-M, Chaix G, Robin C, Mourey N (2009) Procédé de mesure rapide et non destructif des polyphénols du bois de chêne de tonnellerie. Revue Française d'œnologie 234:10–15Google Scholar
- Guitard D (1987) Mécanique du matériau bois et composites. Cépaduès, Toulouse, 238 pGoogle Scholar
- Jeffries TM (2008) Relationships of Growth Rate and Mechanical Properties in Sweetgum, Liquidambar styraciflua. Master. Faculty of the Virginia Polytechnic Institute and State University, Blacksburg, p 107Google Scholar
- Kothiyal V, Raturi A (2011) Estimating mechanical properties and specific gravity for five-year-old Eucalyptus tereticornis having broad moisture content range by NIR spectroscopy. Holzforschung 65Google Scholar
- Love AEH (1892) A treatise on the mathematical theory of elasticity, (edition of 1994) Cambridge University PressGoogle Scholar
- Maeglin RR (1987) Juvenile wood, tension wood, and growth stress effects on processing hardwoods. Applying the latest research to hardwood problems: Hardwood symposium of the Hardwood Research, Memphis, p. 9Google Scholar
- Naes T, Isaksson T, Fearn T, Davies T (2004) A User-friendly guide to Multivariate calibration and classification. NIR Publications, UK, p. 344Google Scholar
- Narayanamurti BD, George J, Pant HC, Singh J (1962) Extractives in Teak. Silvae Genetica 11:57–63Google Scholar
- Nepveu G (1988) Détermination de la qualité du bois par prélèvement non destructif. Revue Forestière Française, n°sp : 62-70Google Scholar
- Pelletier MC, Henson M, Boyton S, Thomas D, Vanclay J (2008) Genetic variation in shrinkage properties of Eucalyptus pilularis assessed using increment cores and test blocks. N Z J For Sci 38:194–210Google Scholar
- Rakotovololonalimanana H (2013) Déterminisme génétique et environnemental des propriétés du bois de Liquidambar styraciflua L. de la Mandraka : adaptation aux reboisements malgaches et apports à la production ligneuse. Thèse de Doctorat, Université de Montpellier 2, Information Structures et Systèmes, Université d’Antananarivo, Ecole Supérieur des Sciences Agronomiques, département des Eaux et Forêts. p. 203Google Scholar
- Rayleigh JWS, Lindsay RB (1877) The theory of sound. (edition of 1945). Dover Publications, New York, pp 243–305Google Scholar
- Sabistina B (2010) Gum : après les paysagistes, il séduit les industriels. Le bois Int 8:15–16Google Scholar
- Saporta G (2006) Probabilité Analyse des données et statistique: France, 619 pGoogle Scholar
- Schimleck LR, Evans R (2004) Estimation of Pinus radiata D. Don tracheid morphological characteristics by near infrared spectroscopy. Holzforschung 58:66–73Google Scholar
- Smith LI (2002) A tutorial on principal components analysis. Cornell University, USA 51: 52Google Scholar
- Zobel BJ & Buijtenen JPv (1989) Wood variation: its causes and control. Springer-VerlagGoogle Scholar